Use of SWIR Imaging to Monitor Layer-To-Layer Part Quality ... ... SWIR imaging data was collected...
Embed Size (px)
Transcript of Use of SWIR Imaging to Monitor Layer-To-Layer Part Quality ... ... SWIR imaging data was collected...
Work performed and funded by The Department of Energy’s Kansas City National Security Campus is operated and managed by Honeywell Federal Manufacturing & Technologies, LLC under contract number DE-NA0002839.
Use of SWIR Imaging to Monitor Layer-to-Layer Part Quality during SLM of 304L Stainless Steel
Cody S. Lough, Xin Wang, Christopher C. Smith, Olaseni Adeniji,
Robert G. Landers, Douglas A. Bristow, Edward C. Kinzel
This paper evaluates using in-situ SWIR imaging to monitor part quality and identify potential defect locations introduced during Selective Laser Melting (SLM) of 304L stainless steel. The microstructure (porosity, grain size, and phase field) and engineering properties (density, modulus, and yield strength) depend on the thermal history during SLM manufacturing. Tensile test specimens have been built with a Renishaw AM250 using varied processing conditions to generate different thermal histories. SWIR imaging data is processed layer-to-layer to extract features in the thermal history for each process condition. The features in the thermal history are correlated with resulting part engineering properties, microstructure, and defects. The use of SWIR imaging is then discussed as a potential for processes monitoring to ensure part quality and develop layer-to-layer control in SLM. This work was funded by Honeywell Federal Manufacturing & Technologies under Contract No. DE-NA0002839 with the U.S. Department of Energy.
Selective Laser Melting (SLM) is a powder bed additive manufacturing (AM) process in
which 3-Dimensional metal parts are produced layer by layer. During SLM, a laser scans and fuses the metal powder bed along paths defined by the part geometry with preset process parameters. The SLM process parameters determine the thermal histories parts experience during manufacturing. The thermal history ultimately controls the microstructure and mechanical properties. Monitoring the thermal history using layer-to-layer infrared imaging gives insight into the SLM process with the potential to ensure part quality.
Researchers have used infrared and visible imaging to understand the thermal history parts
experience during manufacturing and gain information about the melt pool. Long-wave infrared (LWIR) cameras are used to monitor slower dynamics at lower temperatures during SLM. Krauss et al. used a detector sensitive in the LWIR (8-14 μm) to characterize the heat affected zone during SLM of Inconel 718 for variations in laser scan strategies. The detector was used to find and compare off nominal features in the thermal history of the heat affected zone near borders of parts and overhangs. Grasso et al. monitored the SLM process of zinc powder with an infrared camera sensitive from 8-9 μm. The camera was incorporated to monitor the stability of the process and was able to identify the beginning of SLM process failure during layer-to-layer monitoring.
Visible and short-wave infrared (SWIR) cameras are used to monitor faster dynamics in
the SLM process and measure melt pool features. Yadroitsev et al. developed an SLM monitoring system with a CCD camera to measure the surface temperature and melt pool size during processing Ti6Al4V. Findings included the maximum temperature of the melt pool was experienced large increases for processing with higher laser powers, but only small increases for higher exposure times. The width and the depth of the melt pool were determined to scale with
Solid Freeform Fabrication 2018: Proceedings of the 29th Annual International
Solid Freeform Fabrication Symposium – An Additive Manufacturing Conference
changes temperature as a result of processing with varied laser parameters. Heigel and Lane analyzed the effects of powder on the melt pool size and cooling rates experienced during SLM through process monitoring with a SWIR camera. The SWIR imaging data showed an increase in melt pool length and lower cooling rates for processing powder. Cheng et al. used a SWIR camera to monitor melt pool size as a function of build height during SLM of Monel K500. Build height was determined to not significantly affect the melt pool size.
Most researchers use infrared imaging to understand the temperature and size of the melt
pool evolve during manufacturing while some researchers monitor the thermal history to identify defects in the SLM process. In this paper, SWIR imaging is used in layer-to-layer process monitoring during SLM of 304L stainless steel. Thermal features are extracted from the SWIR imaging data to identify defects in 3-Dimensional reconstructions of the SLM parts. These features are related to the melt pool size and SLM process parameters used during manufacturing. The thermal features are then correlated to part engineering properties to understand how data from the thermal history relate to mechanical performance. This is done to ultimately understand if meaningful information can be obtained from the SWIR data to ensure part quality and use in controls oriented decision making.
2. Experimental Setup
A Renishaw AM250 SLM system was used to manufacture cylindrical tensile test
specimens (ASTM E8/E8M) out of 304L stainless steel (layer thickness of 50 µm). The Renishaw AM250 uses a 200 W maximum fiber laser (λ = 1070 nm) that scans with a point-to-point exposure strategy. In the point-to-point exposure strategy, the laser scanning parameters include power, P, exposure time, te, point distance, dp, and hatch spacing, hs. The laser steps along the scan path by the point distance and then emits for the exposure time. To simplify process parameters into a single term, linear energy density, Eρ, can be calculated using Eq. 1.
P tE dρ ⋅
In this work, the tensile specimens were manufactured with constant point distance (60
μm) and hatch spacing (85 μm) while the laser power (100, 125, 150, 175, 200 W) and exposure time (50, 75, 100, 125 µs) were varied. SWIR imaging data was collected in-situ during the SLM manufacturing process for all combinations of laser power and exposure time. Figure 1 (a) is a schematic of the AM250 build chamber with the SWIR camera mounted at a fixed location. The SWIR imaging data was collected through a window installed on the top of the AM250 build chamber. A notch filter was selected to protect the camera from scattered laser radiation and a bandpass filter was utilized to minimize saturation in the thermal data.
FIG 1: (a) Schematic of AM250 building process with SWIR camera observing powder bed and
(b) completed build of tensile test specimens.
Three additional tensile test tensile test specimens were manufactured for layer-to-layer observations using a laser power of 200 W and exposure time of 75 µs. Two of the specimens were manufactured with introduced defects. This was done to demonstrate the ability to detect the defects with in-situ measurements taken with the SWIR camera. A nominal specimen was built for comparison to the defect specimens.
3. Thermal Camera Data Processing
3.1. Thermal Feature Extraction Preforming layer-to-layer observations with the SWIR camera results in time-series data of the laser processing each slice of the tensile test specimen geometry. Figure 2 contains images of the apparent melt pool from selected frames in the time series data for two process parameter combinations. Features can be extracted from this time series thermal data to assign a value to each pixel for compression to a single representative frame for each layer. The pixels in the representative frames have a known size in object space and a third dimension corresponding to the layer thickness can be assigned to create a voxel. A filter for the voxel based data is determined by the thermal feature extracted from the time-series recordings of the layers. In this paper, the time above melt temperature, maximum spatial gradient, and maximum cooling rate are extracted from the time series thermal data for comparison.
Process Laser: P, te
FIG 2: Images of melt pools from SWIR camera data.
In a layer, the time above melt temperature for each pixel is defined as the total time the
pixel is above a set threshold. The melt point threshold was determined by observation of the apparent phase transition region in the spatial profile of a melt pool. Figure 3 (a) is the spatial profile of a melt pool showing the apparent phase transition region corresponding to 12,000 counts. Time above melting temperature is proportionate to the apparent melt pool size. This is explained by the time series data from a pixel in Fig. 3 (b). Due to the raster of the laser during processing the apparent melt pool will pass over a pixel several times for a layer. Larger apparent melt pools results in the pixel measuring values above the melt temperature threshold more times than smaller melt pools. In Fig. 3 (b) the pixel measured values above the apparent phase transition region six times. The time above the melt temperature was increased each time the melt pool passed over the pixel. This means larger time above melt temperature values are proportionate to larger melt pools while smaller values of time above melt temperature correspond to smaller melt pools.
-2.0 -1.5 -1.0 -0.5 0.0 0.5 6000
C o u n ts